Role of Graphene Oxide in Support Layer Modification of Thin Film Composite (
Membrane for Forward Osmosis Application
(Peranan Oksida Grafin dalam Pengubahsuaian Lapisan Sokongan Membran Komposit Filem Nipis (TFC) untuk Aplikasi
Osmosis ke Hadapan)
Wan Nur Syuhada Wan Ata, Ang Wei Lunb & Abdul Wahab Mohammadb*
aChemical Engineering Program, Faculty of Engineering & Built Environment, Universiti Kebangsaan Malaysia, Bangi, Malaysia bResearch Centre for Sustainable Process Technology (CESPRO), Faculty of Engineering & Built Environment,
Universiti Kebangsaan Malaysia, Bangi, Malaysia *Corresponding author: firstname.lastname@example.org
Received 25 January 2019, Received in revised form 16 April 2019 Accepted 17 May 2019, Available online 30October 2019
In this work, the effect of graphene oxide (GO) incorporation into the membrane support layer towards the performance of
thin-film composite (TFC) membrane was investigated. The support layer was fabricated by phase inversion method with the
incorporation of GO as hydrophilic nanoparticles. Next, the active polyamide layer was formed on the membrane support
layer via interfacial polymerization between trimesoyl chloride (TMC) and m-Phenylenediamine (MPD). The cross-section
images from Field-Emission Scanning Electron Microscope (FESEM) showed the presence of active polyamide layer on the
surface of TFC membrane while the FTIR results indicated the existence of bands associated with the amide linkages. The
initial study showed that an optimal amount of GO (0.5 wt%) incorporation into the polymer substrate resulted in favourable
improvement in TFC membrane performance. The physical and chemical properties of GO helps in enhancing the water
transport through the membrane polymer matrix and thus contributing to higher permeate flux. The TFC-FO membrane
incorporated with GO showed 44% improvement in terms of water flux (3.72 compared to 2.09 Lm-2 h-1 for pure PSf membrane)
and minimal improvement in reverse solute diffusion (0.02 compared to 0.03 g m-2 h-1 for pure PSf membrane). Thus, this
study showed that small addition of GO nanoparticles into the membrane support layer leads to an increase in performance
of TFC membrane for FO application.
Keywords: Graphene Oxide; Support Layer; Water Permeation; Thin Film Composite; Forward Osmosis
Kajian ini membentangkan kesan penambahan oksida grafin ke dalam lapisan sokongan membran terhadap prestasi membran komposit filem nipis. Lapisan sokongan membran komposit filem nipis dihasilkan melalui teknik fasa songsang dengan penambahan nanopartikel oksida grafin sebagai nanopartikel bersifat hidrofilik. Seterusnya, lapisan aktif poliamida dihasilkan di atas permukaan lapisan sokongan membran dengan kaedah pempolimeran antara muka menggunakan bahan
kimia trimesil klorida dan m-Fenilenadiamina. Imej keratan rentas dari FESEM membuktikan kehadiran lapisan aktif poliamida
di atas permukaan lapisan sokongan membran komposit filem nipis manakala keputusan FTIR menunjukkan kehadiran
jalur yang dikaitkan dengan jalur amida. Kajian awal menunjukkan bahawa jumlah optimum oksida grafin (0.5 wt%) yang dimasukkan ke dalam substrat polimer menghasilkan peningkatan yang baik terhadap prestasi membran komposit filem nipis. Sifat fizikal dan kimia oksida grafin membantu dalam meningkatkan pengaliran air melalui matriks polimer membran dan seterusnya menyumbang kepada ketelapan air yang tinggi. Membran komposit filem nipis yang telah ditambah oksida
grafin menunjukkan peningkatan sebanyak 44% dari segi fluks air (3.72 berbanding dengan 2.09 Lm-2 h-1 untuk membran
polisulfon tulen) dan sedikit peningkatan dalam penyebaran garam berbalik (0.02 berbanding dengan 0.03 g m-2 h-1 untuk
membran polisulfon tulen). Oleh itu, kajian ini menunjukkan bahawa penambahan oksida grafin ke dalam lapisan sokongan membran menyebabkan peningkatan prestasi membran komposit filem nipis untuk kegunaan osmosis ke hadapan.
Forward osmosis (FO) has been a good alternative to
replace the pressure-driven membrane as it offered valuable advantages including low membrane fouling, high rejections to contaminants and low energy consumption. Since FO is
driven by only osmotic pressure, the energy cost can be lower due to the absence of external hydraulic pressure (McGinnis & Elimelech 2007). Despite all the great advantages that
FO membrane can offer, this process is still facing some
challenges that inhibit its widespread application. The major problem is less availability of good membrane with high water permeation and good rejection properties (Qin, Lay & Kekre 2012).
Recently, researchers have focused on fabricating the thin film composite (TFC) membrane as this type of membrane has
been reported to have a better performance in FO application
as comparison to the cellulose triacetate membrane which is commercially available (Puguan et al. 2014; Wei et al. 2011).
TFC membrane has been modified with several methods in
which one of the methods has gained much attention among the researchers which is modification of the support layer (Bui, Nhu-ngoc and McCutcheon 2013; Hoover, Schiffman & Elimelech 2013). The support layer of TFC membrane
was one of the important parts contributing to the membrane performance as it directly affect the internal concentration polarization (ICP) phenomena in the membrane. The effect of ICP could be tremendous as it could reduce the solute diffusion
rate thoughout the membrane which in turned decrease the water permeability of the membrane. The support layer could be modified by increasing its porosity and hydrophilicity to mitigate the ICP problem in the membrane as per suggested
by (Ma et al. 2013).
Incorporation of nanoparticles into polymeric membrane has gained much attention as one of the ways to enhance the performance of TFC membrane. Titanium dioxide (TiO2)
(Emadzadeh et al. 2014) and modified carbon nanotubes (Wang et al. 2013) have been proven to reduce the ICP effect
in the membrane which improve the membrane performance. In addition to this, porous zeolite nanoparticles have also being incorporated into the membrane support layer (Ma et al. 2013). One of the nanoparticles that gained much attention in improving the properties of membrane was graphene oxide (GO). This nanoparticle offered high surface area-to-volume
ratios which ensure better interaction with polymer matrix as compared to other type of nanoparticles (Stankovich et al. 2006). Up until today, many studies have been conducted on the capability of GO to improve membrane performances.
The water flux of polyvinylidene fluoride (PVDF) membrane
has been significantly increased after GO incorporation due
to the improvement in hydrophilicity of the membrane (Zhao et al. 2013). In another study, it was demonstrated that GO
nanoparticles could act as a modifier which not only improve the water flux but also result in increase in antifouling property (Wang et al. 2012). PES/GO membrane was also shown to have
higher water permeation and better antifouling properties with GO incorporation compared to the pure PES membrane
(Zinadini et al. 2014). In addition to that, GO had been used in
fabricating FO membrane which improve the water permeation
and antibacterial properties of the membrane. Several recent works which reported the incorporation of GO including study
by Soroush et al. (2015), which covalently bonded GO/Ag
nanocomposites to the TFC polyamide membrane surface to
produce superhydrophilic membranes whereas Perreault et al. (2016) proved that the biofouling problem in FO membrane had
reduced after incorporation of GO into TFCFO membrane by
amine coupling reaction. In addition to this, a study reported a polyamide-graphene oxide FO membrane which was fabricated
by cross-linking of GO aggregates with m-xylylenediamine
(MXDA) and trimethyle chloride (TMC) also exhibited high
water flux (Jin et al. 2018).
Eventhough GO has proven to improve the membrane
performance including FO membrane, many conducted
studies were only focusing on the surface modification of
TFC membrane which somehow involves the changes in the
polyamide active layer only. Up to date, there was still limited study being done on the support layer modification of TFC
membrane by incorporation of GO nanoparticles. Hence, this
study was conducted to investigate the role of GO in enhancing
the performance of TFC membrane.
Graphite powder and N,N-Dimethylacetamide (DMAc) were
purchased from Merck (Germany) while sulfuric acid (H2SO4) were from Accot (Malaysia). Potassium permanganate (KMnO4), 1,3,5-Benzenetricarbonyl trichloride (TMC) and
m-Phenylenediamine (MPD) were obtained from Sigma Aldrich
(USA). Polymer, polysulfone (PSf) was from GoodFellow (UK).
Hexane and sodium chloride (NaCl) were supplied by R&M
(Malaysia). All the solutions were prepared with deionized water (DI).
Modified Hummer’s Method has been used to synthesis GO
in laboratory scale as being described clearly in one of the previous study by (Mahmoudi et al. 2015).
SUPPORT LAYER FABRICATION
Phase inversion technique was devoted to fabricate PSf and PSf/GO by using DMAc as a solvent. PSf was dissolved into
the solvent at weight composition of 18:82 respectively as a casting solution. Different wt% of GO with respect to PSf
which ranging from 0.1-1.0 wt% were dissolved into the casting solution and was continously stirred at 300 rpm for overnight to form a homogenous solution. Then, the solution was kept unstirred in the dessicator for another overnight. Before fabrication, the casting solution was sonicated for 30 minutes. The casting solution was casted with Elcometer 4340 Automatic Film Applicator available in the laboratory with
the casting thickness of 200 µm. Immediately, the glass plate was immersed horizontally in the ultrapure water after being exposed to air for 15 secs. The membranes fabricated were denoted as pure PSf, PSFGO-0.1, PSfGO-0.25, PSfGO-0.5,
PsfGO-0.75 and PSfGO-1.0, according to the amount of GO
incorporated into it.
INTERFACIAL POLYMERIZATION OF TFC FO MEMBRANE The membrane was air-dried for overnight before the procedure was started. The membrane was taped nicely on a glass plate before being immersed for 2 minutes in the 2% MPD solution. Finally, the membrane was immersed in
0.1% TMC/hexane for 1 minute. The membrane was kept in
a container filled with DI water for futher testing (Low et
CHARACTERIZATION AND ANALYTICAL METHODS
Functional groups of GO was analyzed by using FTIR
spectrometer (Thermo Fisher Scientific Inc., USA) and the
crystallinity of GO was tested by XRD (Bruker D8 Advance,
Germany). The changes in the morphology of the membrane support layer was viewed by using Field-Emission Scanning Electron Microscope (Gemini model SUPRA 55VP-ZEISS,
Germany). The roughness analysis were done by Atomic Force Microscopy (NTEGRA Prima, NT-MDT, Russia). The
surface hydrophilicity of membrane support layer were analyzed using a Drop Shape Analysis System goniometer.
WATER PERMEABILITY TEST
Membrane permeability was tested with dead end unit available in the laboratory. Membrane has been pressurized to 10 bar for an hour to reduce the membrane compaction effect before the test started. The stirring speed was set to 300 rpm. Then, membrane was pressurized with different pressure 2,4,6,8 and 9 bar for water permeability test. Membrane permeability can be obtained from the graph of permeate flux against operating pressure. The permeate flux of the support membrane was obtained by using this equation:
where J (L/m2 h) is permeate flux, V is the permeate volume
(L), A is the membrane effective area (m2) and t is the time
of testing (h) (Low et al. 2015).
TFC FO MEMBRANE PERFORMANCE EVALUATION
FO system with a Sterlitech CF042 cell measuring 12.7 cm ×
10 cm × 8.3 cm was used to evaluate the performance of TFC
membrane. The active layer of TFC membrane was set to face
the feed solution. 1 L of DI water was used for feed solution while 0.5 L of NaCl (1M) was used for draw solution with the fact that the volume of a solution has no significant effect on the water flux in forward osmosis membranes as been mentioned in previous study by (Law & Mohammad 2017)
Both solution was circulated in a closed loop counter-current by aid of two peristaltic pump (BT600-2J, LongerPump,
China). A digital balance was used to record the weight changes in draw solution as illustrated in Figure 1 below:
FIGURE 1. Bench scale FO system diagram
Finally, the water permeation flux, Jw can be obtained
by this equation: m J A t ∆ = ∆ r (2)
where Δm (g) is the weight of permeate water, Δt (h) is the testing duration, ρ is the density of water and A is the effective area of membrane (m2) (Low et al. 2015). The
salt leakage usually referred to reverse salt diffusion from the draw solution to the feed solution was determined from conductivity measurements using a calibration curve for the NaCl2 solution. The reverse salt diffusion flux (Js in gm-2h-1,
abbreviated as gMH) was thereafter determined from the increase of the feed conductivity value using this formula:
( s t) 1 s c v J t A ∆ = ∆ (3)
where Cs and Vt are the salt concentration and the volume of
the feed in the end of FO tests, respectively.
RESULTS AND DISCUSSION
XRD ANALYSIS OF GO
The oxidization of graphite into graphene oxide was confirmed with XRD analysis. The XRD patterns obtained for
graphite and synthesized GO are shown in Figure 2. Graphite
exhibited a strong peak at 26.575° with interlayer distance of 0.335 nm. Meanwhile, as can be seen in Error! Reference
source not found., GO exhibited a peak at 10.787° with
interlayer distance of 0.82 nm which showed that graphite was completely oxidized into GO after the chemical oxidation
process. Similar findings were observed by other work (Junaidi et al. 2018; Zakaria et al. 2018), where GO exhibited
FTIR ANALYSIS OF GO
Based on the observation of the IR-spectrum of graphite in Figure 3, the O-H stretch can be seen at the peak at 3610 cm-1
while the peak at 1677 cm-1 was due to the C = C vibration
(Ganesh, Isloor & Ismail 2013) changes in FT-IR spectra of
graphite was obvious after it was fully oxidized into GO as
being shown in Figure. The strong C = O stretch can be seen in GO spectra at 1621 cm-1. Other than that, the peak near 3565
cm-1 was due to the O-H stretching vibrations whereas peak
at 1224 cm-1 and 1417 cm-1 were formed from the vibrations
of epoxy C-O and C-OH respectively. The FT-IR results
showed that the oxygen functional groups were successfully established onto the graphite surface during the oxidation reaction, which produced the desirable GO products. This
result was consistent with the findings by other researchers (Haan et al. 2018; Rezaee et al. 2015).
CHARACTERIZATION OF MEMBRANE SUPPORT LAYER
FESEM images in Figure 4 showed the membrane morphology
after incorporation of GO nanoparticles. Pure PSf membrane
tends to have a few macrovoids with spongy structure at the bottom part of the membrane. On the other hand, after GO has
been added at concentration of 0.1, 0.25 and 0.5 wt%, more macrovoids were present and spongy structure was reduced. The morphology of membrane has changed as GO loading
was increased, more macrovoids were present and reduce the spongy structure. The incorporation of GO increased the
speed of phase inversion process in which such modification causes the formation of microvoid and a spongy structure in the membrane as mentioned by many other works (Chung et al. 2017; Wang et al. 2012). Similar observation has been reported previously by Zinadini et al. (2014), where porosity of nanofiltration (NF) membrane increased with increasing GO content. This was supported by some studies which
revealed that the membrane porosity has been increased after incorporation of GO due to the formation of larger finger-like
voids (Wang et al. 2015).
FIGURE 2. The XRD patterns for graphite and GO synthesized FIGURE 3. FT-IR spectra of graphite and GO synthesized
AFM was conducted to evaluate the surface roughness
of the fabricated membrane support. Based on Figure 5, it can be seen that the dark areas represented the pores of the membranes. It was revealed that the pure PSf membrane support exhibited average roughness, Ra = 7.034 nm and root mean square of surface roughness, Rms = 8.931 nm. Meanwhile, PSF/GO membrane support exhibited sharper and
denser asperities in comparison to the pure PSf membrane. Particularly, as GO loading has been increased to 0.5 wt%, the
roughness values were decreased and increased again at GO
loading greater than 0.5 wt%. The presence of GO has proven
to reduce the surface roughness of PSf/GO, which can be seen
in the roughness value at GO-0.5. This was due to the fact that
at low concentration of GO, the low electrostatic interactions
among the GO resulted in collocation in membrane leading to
smoother surface of the membrane. Hence, it could reduce the membrane roughness and thus creating smooth surface (Qiu et al. 2009).
FIGURE 5. The three dimentional surface morphology of the prepared membrane support The membrane hydrophilicity has been analyzed by
contact angle test. As being reported in Figure 6 below, the contact angle of pure PSf membrane was 82° and was significantly reduced to 66º when 0.5 wt% has been added into the membrane support layer. This has been also proven by many previous research works which reported that membranes showed lower contact angle after incorporation of hydrophilic nanomaterials (Y. Wang et al. 2013; Xu et al. 2014; Zinadini et al. 2014). The presence of oxygenous functional groups such as hydroxyl, epoxy groups and carboxyl groups in GO
has increase the hydrophilicity of the membrane. This was supported by a study conducted by Zhao et al. (2013) which reported that the addition of graphene to the PVDF membrane
improved the surface hydrophilicity and pure water flux of the membrane On the other hand, the incorporation of GO into the PES membrane has been investigated by Zinadini et al. (2014)
in which their membranes showed significant improvement in water flux due to the increasing hydrophilicity of the membrane. However, further increase of GO wt% greater
than 0.5 wt% has increased the contact angle value. This phenomena happened as incorporation of higher GO loading
resulted in higher viscosity of casting solution which in turned, reduced the membrane pore size and porosity as explained by (Rezaee et al. 2015) in one of their publications. The viscous casting solution may delay the exhange rate between solvent and non-solvent. Some studies reported that
in this situation, the decrease in hydrophilicity of membrane might be due to the pore blockage by high concentration of
GO (Wang et al. 2012).
The water permeability of the membrane support started to increase when GO has been incorporated as comparison
to the pure PSf membrane as can be seen in Figure 7. Unfortunately, further increase of GO addition at 0.75 and 1.0
wt% significantly reduce the water permeation through the membrane. This could be due to the irregular placement of GO
particles in the membrane (Vatanpour et al. 2011). In addition to this, the water permeation reduction with GO addition
more than 0.75 wt% could be due to the pore blockage by high concentration of GO as being observed by other studies
(Vatanpour et al. 2011; Wang et al. 2012).
reported previously which revealed that at 0.5 wt% of GO, the
water permeation and hydrophilicity of membrane has been increased significantly. In this section, the performance of TFC FO-GO has been compared with the pure TFC FO membrane
In FO mode, the modified membrane (TFC FO-GO) showed
higher water flux, Jw in which it was increased by 44%
compared to the pure TFC FO as reported in Table 1 below.
In addition to this, reverse salt diffusion was studied as the draw solute leakage through the membrane may affect the osmotic pressure gradient across the membrane. As being reported in Table 1, the TFC FO-GO membrane recorded
relatively lower reverse salt diffusion compared to the pure
TFC FO membrane. The increase in water flux of TFC FO-GO
membrane was due to the physical and chemical properties of GO, which enhance the water permeation through the
membrane (Gao, Hu & Mi 2014). Water molecules can physically be transported via the GO nanosheet channels, and
chemically GO helps in water molecules adsorption into the
membrane due to its hydrophilic functional groups (hydroxyl, carboxyl and epoxy). This is proven by the contact angle result below. The contact angle has been reduced from 68° to 53° after incorporation of GO into the TFC FO membrane
which indicates that GO has improved the hydrophilicity of TFC FO membrane.
FIGURE 6. Contact angle for different type of membrane based on GO wt%
FIGURE 7. Water permeability of membrane support layer
0 W ater Permeability (L.m -2.hr -1.bar -1) 0 1 2 3 4 0.1 0.25 0.3 GO wt% 0.5 0.75 1
PERFORMANCE EVALUATION OF TFC FO MEMBRANE
TFC FO membrane was fabricated with incorporation of
optimal concentration of 0.5 wt% GO and denoted as TFC FO-GO. This concentration was chosen owing to the results
from the characterization of membrane support layer as being
TABLE 1. Water flux, reverse salt diffusion and contact angle of
both TFC membranes
Membrane Water Flux, Reverse Salt Contact Angle Type Jv (L m-2h-1) Diffusion (g m-2 h-1) (°)
TFC FO 2.1 0.03 68.20.1
TFC FO-GO 3.7 0.02 53.30.4
Based on the FESEM images in, the presence of polyamide
active layer can be seen by the formation of ridge and valley structures on the membrane surface and via the top cross-section images of TFC FO-GO membrane (Ma et al. 2012). This
was supported by the FTIR result in Figure 9. The presence
of polyamide layer was confirmed by the existence of bands associated with amide linkages. The carbonyl vibrations exhibited a peak at 1667 cm-1 , while the amide II band can
be seen at peak 1585 cm-1 which is due to the N-H bending
and C-N vibrations of the amide group (Belfer, Gilron & Kedem 1999). Amide linkages was formed as can be seen by the peak exhibited at 1667 cm-1 due to the reaction of
-COOH group from GO with NH2 group from MPD (Saha &
Joshi 2009). This result has proven the presence of polyamide layer on the surface of TFC membrane.
In conclusion, it is believed that the performance of TFC
membrane was directly affected by the properties of its support layer. The optimum amount of GO (0.5 wt%)
the water permeation of TFC membrane by 44% compared
to the pure TFC membrane. This study has proven that the
incorporation of hydrophilic nanoparticle of GO into the
membrane support layer can be a good approach in order to develop an effective TFC FO membrane.
The author gratefully acknowledges the financial support by Ministry of Education Malaysia (LRGS/2013/UKM-UKM/ PT/03) for funding this study.
Belfer, S., Gilron, J. & Kedem, O. 1999. Characterization of commercial RO and UF modified and fouled membranes by means of ATR/FTIR. Desalination 124(1-3): 175-180.
Bui, N.-N. & McCutcheon, R.J. 2013. Hydrophilic nano fibers as new supports for thin film composite membranes for engineered osmosis. Environmental Science &
Technology 47: 1761-1769.
Chung, Y.T., Mahmoudi, E., Mohammad, A.W., Benamor, A., Johnson, D. & Hilal, N. 2017. Development of polysulfone-nanohybrid membranes using ZnO-GO composite for enhanced antifouling and antibacterial control. Desalination 402: 123-132.
Emadzadeh, D., Lau, W.J., Matsuura, T., Ismail, A.F. & Rahbari, M.-S. 2014. Synthesis and characterization of thin film nanocomposite forward osmosis membrane with hydrophilic nanocomposite support to reduce
internal concentration polarization. Journal of Membrane
Science 449: 74-85.
Ganesh, B.M., Isloor, A.M. & Ismail, A.F. 2013. Enhanced hydrophilicity and salt rejection study of graphene oxide-polysulfone mixed matrix membrane. Desalination 313: 199-207.
Gao, Y., Hu, M. & Mi, B. 2014. Membrane surface modification with TiO2-graphene oxide for enhanced photocatalytic performance. Journal of Membrane
Science 455: 349-356.
Haan, T.Y., Rosnan, N., Adilah & Mohammad, A.W. 2018. Synthesis and Characterization of ZnO-decorated GO Nanocomposite Material with Different ZnO Loading through Sol-gel Method. Jurnal Kejuruteraan 30(2): 249-255.
Hoover, L.A., Schiffman, J.D. & Elimelech, M. 2013. Nanofibers in thin-film composite membrane support layers: Enabling expanded application of forward and pressure retarded osmosis. Desalination 308: 73-81. Jin, L., Wang, Z., Zheng, S. & Mi, B. 2018.
Polyamide-crosslinked graphene oxide membrane for forward osmosis. Journal of Membrane Science 545: 11-18. Junaidi, N.F.D., Khalil, N.A., Jahari, A.F., Shaari, N.Z.K.,
Shahruddin, M.Z., Alias, N.H. & Othman, N.H. 2018. Effect of Graphene Oxide (GO) on the Surface Morphology & Hydrophilicity of Polyethersulfone (PES). IOP Conference Series: Materials Science and
Engineering 358(1): 1-6.
Law, J.Y. & Mohammad, A.W. 2017. Assessing the forward osmosis performances using CTA membrane: Effect of solution volume ratio and type of draw solute. Jurnal
Teknologi 79(5-3): 47-52.
Low, Z.X., Liu, Q., Shamsaei, E., Zhang, X. & Wang, H. 2015. Preparation and characterization of thin-film composite membrane with nanowire-modified support for forward osmosis process. Membranes 5(1): 136-149.
Ma, N., Wei, J., Liao, R. & Tang, C.Y. 2012. Zeolite-polyamide thin film nanocomposite membranes: Towards enhanced performance for forward osmosis. Journal of Membrane
Science 405-406: 149-157.
Ma, N., Wei, J., Qi, S., Zhao, Y., Gao, Y. & Tang, C.Y. 2013. Nanocomposite substrates for controlling internal concentration polarization in forward osmosis membranes. Journal of Membrane Science 441: 54-62.
Mahmoudi, E., Ng, L.Y., Ba, M.-A.M. & Mohammad, A.W. 2015. Novel nanohybrid polysulfone membrane embedded with silver nanoparticles on graphene oxide nanoplates. Chemical Engineering Journal 277: 1-10. McGinnis, R.L. & Elimelech, M. 2007. Energy requirements of
ammonia-carbon dioxide forward osmosis desalination.
Desalination 207(1-3): 370-382.
Perreault, F., Jaramillo, H., Xie, M., Ude, M., Long, D.N. & Elimelech, M. 2016. Biofouling Mitigation in Forward Osmosis using Graphene Oxide Functionalized Thin-Film Composite Membranes: Supporting Information. FIGURE 8. Surface and cross section FESEM image of TFC FO-GO
Environmental Science & Technology 50(11):
Puguan, J.M.C., Kim, H.S., Lee, K.J. & Kim, H. 2014. Low internal concentration polarization in forward osmosis membranes with hydrophilic crosslinked PVA nanofibers as porous support layer. Desalination 336: 24-31. Qin, J.J., Lay, W.C.L. & Kekre, K.A. 2012. Recent
developments and future challenges of forward osmosis for desalination: A review. Desalination and Water
Treatment 39(1-3): 123-136.
Qiu, S., Wu, L., Pan, X., Zhang, L., Chen, H. & Gao, C. 2009. Preparation and properties of functionalized carbon nanotube/PSF blend ultrafiltration membranes. Journal
of Membrane Science 342(1-2): 165-172.
Rezaee, R., Nasseri, S., Mahvi, A.H., Nabizadeh, R., Mousavi, S.A., Rashidi, A., Jafari, A. & Nazmara, S. 2015. Fabrication and characterization of a polysulfone-graphene oxide nanocomposite membrane for arsenate rejection from water. Journal of Environmental Health
Science and Engineering 13(1): 1-11.
Saha, N.K. & Joshi, S.V. 2009. Performance evaluation of thin film composite polyamide nanofiltration membrane with variation in monomer type. Journal of Membrane
Science 342(1-2): 60-69.
Soroush, A., Ma, W., Silvino, Y. & Rahaman, M.S. 2015. Surface modification of thin film composite forward osmosis membrane by silver-decorated graphene-oxide nanosheets. Environmental Science: Nano 2: 395-405. Stankovich, S., Dikin, D.A., Dommett, G.H.B., Kohlhaas,
K.M., Zimney, E.J., Stach, E.A., Piner, R.D., Nguyen, T.S. & Ruoff, R.S. 2006. Graphene-based composite materials. Nature 442: 282-286.
Vatanpour, V., Madaeni, S.S., Moradian, R., Zinadini, S. & Astinchap, B. 2011. Fabrication and characterization of novel antifouling nanofiltration membrane prepared from oxidized multiwalled carbon nanotube/polyethersulfone nanocomposite. Journal of Membrane Science 375(1-2): 284-294.
Wang, Y., Ou, R., Ge, Q., Wang, H. & Xu, T. 2013. Preparation of polyethersulfone/carbon nanotube substrate for high-performance forward osmosis membrane. Desalination 330: 70-78.
Wang, Y., Ou, R., Wang, H. & Xu, T. 2015. Graphene oxide modified graphitic carbon nitride as a modifier for thin film composite forward osmosis membrane. Journal of
Membrane Science 475: 281-289.
Wang, Z., Yu, H., Xia, J., Zhang, F., Li, F., Xia, Y. & Li, Y. 2012. Novel GO-blended PVDF ultrafiltration membranes. Desalination 299: 50-54.
Wei, J., Qiu, C., Tang, C.Y., Wang, R. & Fane, A.G. 2011. Synthesis and characterization of flat-sheet thin film composite forward osmosis membranes. Journal of
Membrane Science 372(1-2): 292-302.
Xu, Z., Zhang, J., Shan, M., Li, Y., Li, B., Niu, J., Zhou, B. & Qian, X. 2014. Organosilane-functionalized graphene oxide for enhanced antifouling and mechanical properties of polyvinylidene fluoride ultrafiltration membranes.
Journal of Membrane Science 458: 1-13.
Zakaria, Z., Shaari, N. & Kamarudin, S.K. 2018. Preliminary Study of Alkaline Direct Ethanol Fuel Cell by using Crosslinked Quaternized Poly (Vinyl Alcohol)/Graphene Oxide Membrane. Jurnal Kejuruteraan 30(2): 219-227.
Zhao, C., Xu, X., Chen, J. & Yang, F. 2013. Effect of graphene oxide concentration on the morphologies and antifouling properties of PVDF ultrafiltration membranes. Journal of
Environmental Chemical Engineering 1(3): 349-354.
Zinadini, S., Zinatizadeh, A.A., Rahimi, M., Vatanpour, V. & Zangeneh, H. 2014. Preparation of a novel antifouling mixed matrix PES membrane by embedding graphene oxide nanoplates. Journal of Membrane Science 453: 292-301.